Composites of Bacterial cellulose
As is well-known, cellulose is one of the most abundant biodegradable materials in nature and has been the topic of extensive investigations in macromolecular chemistry. It is of great importance to explore renewable natural polymeric materials to solve problems such as population growth, the energy crisis, environment polution, etc. Presently, human beings can produce cellulose by four means. Two of these are by natural synthesis procedures including plant photosynthesis and microbial synthesis. The other two methods are synthetic and enzymatic synthesis from cellobiose fluoride
Bacterial cellulose (BC, also known as microbial cellulose, MC) is a promising natural polymer synthesized by certain bacteria. Because of its unique structural and mechanical properties as compared to higher plant cellulose, BC is expected to become a commodity material in various fields. The BC fibers have a high aspect ratio with a diameter of 20-100 nm. As a result, BC has a very high surface area per unit mass. This property, combined with its highly hydrophilic nature, results in a very high liquid loading capacity. Morever, biocompatibility makes it an attractive candidate for a wide range of applications in different fields, especially those related to biomedical and biotechnology applications (Dahman, 2009). The fibrous structure of BC consists of a three-dimensional non-woven network of nanofibrils, sharing the same chemical structure as plant cellulose, which is held together by inter- and intra-fibrilar hydrogen bonding resulting in a never-dry hydrogel state with high strength.
The biosynthetic pathways of BC, including those involving enzymes and precursors, have been described (Chawla et al., 2009). These cellulosic materials are particularly attractive because of their relatively low cost and plentiful supply. Thus, BC utilization is responsible for one of the largest material flows in the biosphere and is of interest in relation to the analysis of carbon flux at both local and global scales (Lynd et al., 2002). Plenty of work has been devoted to designing ideal biomedical devices from BC. Such devices are advantageous in terms of their high paper-like reflectivity, flexibility, contrast, and biodegradability (Iguchi et al., 2000, Klemm, 2006). Besides, BC has proven to be a remarkably versatile biomaterial and can be used in a wide variety of products such as paper, electronics, acoustics and so on. Cellulose has always been the prime medium for displaying information in our society and is far better than the various existing display technologies. The BC device has the potential to be extended to countless other applications such as e-book tablets, e-newspapers, dynamic wall papers, rewritable maps, and learning tools (Shah, 2005). Olsson et al. used freeze-dried bacterial cellulose nanofibril aerogels as templates to make lightweight porous magnetic aerogels, which can be compacted into a stiff magnetic nanopaper (Olsson et al., 2010). As intuitionistic introduction, the biomedical applications of BC are shown in Figure 1.
However, in most practical applications, BC may not be of perfect quality and its cost may not be suituable for industrialization either. For economical mass production, it is essential to design a culture aeration and agitation process (Yoshinaga, 1997; Yamanaka, 1998). This chapter will discuss the biosynthesis of BC and its application as skin tissue repair material. The skin tissue materials derived from BC may create a luciferous future.
In this chapter, we focus on the applications of BC as skin tissue repair materials. Specifically, we summarize the basic properties, different types of BC, and research on BC for the purpose of applying BC to skin tissue engineering. Experimental results and clinical treatments have demonstrated good performance of BC-based wound healing materials. Further, all the results indicate that BC as skin tissue material in the biomedical field will continue to be important in the future.
2. Structure and properties of Bacterial Cellulose
2.1. Structure of BC
Based on X-ray investigations, the orientational state of polymers in general can be defined. BC membranes exhibit uniplanar orientation and an additional axial orientational component that depends on the drying procedure. It is possible to produce uniplanar-axial orientation by drawing, the degree of uniplanar and especially uniaxial orientation depending on the drawing conditions (Bohn et al., 2000). In 1984, VanderHart & Atalla investigated various cellulose samples by Nuclear Magnetic Resonance (NMR) spectroscopy and found that all natural cellulose was a complex of both Iα and Iβ forms, and the content of Iα was about 65% in BC (VanderHart & Atalla, 1984). The study of Hirai et al. showed that decreased Iα-cellulose content led to smaller microfibrils in BC (Hirai et al., 2009). Generally, a uniplanar texture with the planes parallel to the fiber surface and an axial component in the drawing direction were found. As compared to wet aqueous samples, a higher coherent deformation of BC can be achieved by soaking the samples in NaOH solutions with concentration ranging from 8 to 10 wt %. In the presence of lye, significant improvement (up to 100%) in axial chain orientation can be obtained, resulting in a maximum strength of 580 MPa. Improved orientability is likely due to a NaOH-induced reduction in the number of inter-fibrillar bridging points formed by H-bonds (Bohn et al., 2000).The analysis based on the simple spin diffusion theory for the process experimentally observed reveals that the upfield carbons may be located at a distance less than about 1 nm from the downfield carbons in 13C spin diffusion measurements. It was found that the downfield and upfield carbons were almost equally subjected to 1H spin diffusion from the poly (vinyl alcohol) phase, indicating that the upfield carbons were not localized in some limited area, e.g. in the surfacial region, but were distributed throughout the whole area in the microfibrils. These experimental results suggested that the C4U carbons might exist as structural defects, probably due to conformational irregularity associated with disordered hydrogen bonding of the CH2OH groups in the microfibrils (Masuda et al., 2003).
2.2. Characterization of bound water
BC is a gel containing 99% of water by weight, mainly due to its amorphous structure. Unfortunately, comparing the water holding capacities of different BC samples is difficult because different methods have been used. Drying under vacuum (10 mm H2O or 98 Pa) was found to be preferable to stabilize the sample prior to determining its wet weight. This simple method lowered the standard deviation on the measurements by 50% or more as compared to other methods (Schrecker & Gostomski, 2005). According to dielectric spectroscopy and electron microscopy, the majority of the water molecules is tightly bound to BC, while only 10% out of the 99 wt% water presenting in BC gels behaves like free bulk water (Gelin et al., 2007).
The sorption properties of BC gel films were studied by Baklagina et al. The crystal structure of BC remained unchanged when polyvinylpyrrolidone or its complex with silver nanoparticles was incorporated into its matrix. By washing with distilled water, polyvinylpyrrolidone was readily removed from composite gel films of BC and polyvinylpyrrolidone or Poviargol without causing any changes in the cellulose structure and the amount of the adsorbed silver (Baklagina et al., 2005).
2.3. Mechanical properties
Recent studies have shown that atomic force microscopy can be used to measure the elastic modulus of suspended fibers by performing a nanoscale three-point bending test, in which the center of the fiber is deflected by a known force. By calculating the displacement with respect to the applied strain, it was shown that the stiffness of a single fibril of BC could be estimated. To demonstrate this concept, Guhados et al. have measured Young modulus of BC fibers with diameters ranging from 35 to 90 nm at a value of 78 ± 17 Gpa. This value was considerably higher than previous estimates obtained from the mechanical strength of individual cellulose fibers (Guhados et al., 2005). The modulus was also predicted from a calibration curve for a Raman band shift against modulus, based on previously published data, and by using Krenchel analysis to back-calculate the modulus of a single fibril. The value obtained (114 GPa) was higher than those reported previously, but lower than estimates from the modulus of crystalline cellulose-I (130-145 GPa) (Hsieh et al., 2008).
The fermentation time had a large effect on both the number of bacteria and the cellulose yield, but only minor effects on the mechanical properties, indicating that the fermentation technique is a robust method for the production of cellulose with predictable properties. A study by McKenna et al. showed that an increase in the fermentation time could led to a decrease in mechanical strength, Young’s modulus first increasing and then decreasing after 96 h. Treatment with NaOH had minimal effects on the mechanical properties. The failure zone in uniaxial tension was shown to be associated with large-scale fibre alignment, this being a major determinant of mechanical properties. As was expected, the elastic modulus and failure stress under uniaxial tension were one order of magnitude lower than the values obtained under biaxial tension, since a fibre alignment mechanism is not available under biaxial tension. BC behaves like a viscoelastic material, brittle failure being reached at approximately 20% strain and 1.5 MPa stress under uniaxial tension (McKenna et al., 2009). Compression pressure has been found to be an important parameter controlling the final mechanical properties of BC films: Slightly enhanced tensile strength and deformation at break were obtained by increasing the molding compression pressure, while the modulus also decreased nearly linearly with increasing film porosity. This behavior was related to higher densification under the increased mold compression pressure which reduced the interfibrillar space, thus increasing the probability of interfibrillar bonding (Retegi et al., 2010).
2.4. Rheology properties
Rheological analysis was developed to evaluate the fibril width and length of disintegrated BC. During the early stage of the disintegration process, the BC particles formed loose fibrous aggregates, followed by cutting of the disintegrated fibrils that produced short fibrils. On the other hand, the fibril width decreased steadily throughout the disintegration process. The relationships between fibril structure and suspension properties were analyzed. The thinner and longer the disintegrated bacterial cellulose fibrils were, the higher the viscosity and water-holding capacity became (Ougiya et al., 1998).
To characterize the mixing of BC culture broth, which can affect the productivity of BC, non-Newtonian behavior during mixing of a 1% BC suspension was studied using an image processor capable of detecting color changes for a pH indicator and was compared with that of a 2% carboxy methyl cellulose (CMC) solution. The CMC solution was mixed homogeneously within the measured range of agitation speeds, while the BC suspension was not homogeneously mixed at agitation speeds lower than 15 rps because mixing was delayed in some areas of the vessel. A possible reason for the inhomogeneity of the BC suspension at low agitation speeds is the non-Newtonian behavior which increases viscosity at low shear rates (Kouda et al., 1996).
For the three kinds of cellulose solutions, the values of 0 - s (0: zero-shear viscosity of the solution, s: solvent viscosity) were in proportion to the weight fraction of polymer, w, in the dilute solution regime. The plateau modulus, GN, was proportional to w 2 for Cotton linter solutions, signifying that an entangled network structure was formed in the cotton linter solution, as is often observed for solutions of flexible synthetic polymers. On the other hand, the concentrated solution of BC typically displayed small-angle X-ray scattering (SAXS) profiles typical of two-phase systems (Tamai et al., 2003).
3. Bio-fabrication of Bacterial Cellulose
Biodegradable composites made entirely from renewable resources are urgently sought after to improve material recyclability. Many biobased polymers and natural fibers usually display poor interfacial adhesion in composite materials. To modify the surface of natural fibers, BC was utilized as substrates for bacteria during fermentation of BC (Pommet et al., 2008).
The fabrication of a BC network sheet was attempted by heat-pressing in metal molds with a micro pattern to open a pathway to potentially versatile materials. A structural hydrophobic similar to the "Lotus effect" on this sheet was thus examined by introducing a micro-lattice pattern onto its surface. Indeed, the surface of the sheet was found to be more hydrophobic when the structural hydrophobic effect and the synergistic effects of heating and micro-patterning were combined (Tomita et al., 2009).
3.1. Self-assembled and oriented Bacterial Cellulose
Potato and corn starch were added to the culture medium and partially gelatinized in order to allow BC nanofibrils to grow in the presence of a starch phase. The BC-starch gels were hot pressed into sheets with a BC volume fraction higher than 90%. During this step, starch was forced to further penetrate the BC network. The self-assembled BC-starch nanocomposites displayed coherent morphologies (Grande et al., 2009).
Since the oxygen produced by the electrolysis of water in the culture media is far from the liquid-air boundary, aerobic cellulose production into 3D structures is readily achievable. Five separate sets of experiments were conducted to demonstrate the assembly of nanocellulose by
The effect of agar plates on BC production in a static culture medium was investigated in order to reveal the role of the agar component as a surface-modifying agent. The maximum water holding capacity value 92.21 g/g was measured for BC formed in reactors modified with 3.0% of agar. The maximum production rate was observed after the second day of cultivation as compared to the third day of cultivation in the case of the control experiment without agar (Shah et al., 2010).
BC with an unoriented microfibril network forms at the air-liquid interface (BC-air), while BC gel can be produced on an oxygen-permeable substrate such as polydimethylsiloxane (PDMS). The gel thus obtained shows strong birefringence with colorful images in polarized light microscopy, which is typical of liquid crystal-like structures. The optimum ridge size of 4.5 μm was related to the contour length of the bacteria cells. The fracture stress () of uniaxially oriented BC gel under elongation was 4.6 MPa, which was 2.3 times higher than that of the BC-air material ( = 2 MPa) (Putra et al., 2008).
The extraction and refinement of high-strength crystalline microfibril bundles (15-20 nm thick) from BC networks was investigated, as well as their morphology prior to and post electrospinning. The diameter of the fibers decreased significantly with increasing cellulose contents from about 1.8 m (1 wt %) to about 100 nm (20 wt %). The nominal content of cellulose in the fibers was assessed by Lorentzian profile fit assignment of the crystalline phase, and the results showed significantly improved thermal stability for the composite material. The fibers were aligned into an anisotropic nanocomposite during spinning (Olsson et al., 2010).
3.2. Magnetic Bacterial Cellulose
Uniform magnetic membranes can be obtained from microfibrillar bacterial cellulose suspensions loaded with nanosized ferrites (mainly magnetite). The cellulose microfibrils act as a nucleation site for the growing ferrites (Sourty et al., 1998). Ferrites were thus synthetized in situ in two different neutral cellulose gels: a never-dried bacterial cellulose membrane and a never-dried film cast from N-methylmorpholine-N-oxide. The results showed the presence of ferrites in two different shapes, acicular and equiaxial, respectively corresponding to hydrated ferric oxides (FeOOH) and the spinel oxides (maghemite, -Fe2O3, or magnetite, Fe3O4). Thin sections of bacterial cellulose showed that these particles were located along the cellulose microfibrils, which were assumed to provide sites for the nucleation of these particles. Room temperature magnetization curves showed that all the samples were superparamagnetic (Sourty et al., 1998). Bacterial cellulose, with its porous network structure, was also used as an accelerator to precipitate Ni nanoparticles by the room temperature chemical reduction of NiCl2 hexahydrate. Interestingly, BC did not undergo any change and retained its crystal structure even after the chemical reduction reaction. The fraction of isolated superparamagnetic nanoparticles present in the composite was estimated from the saturation magnetization and found to be around 88% (Vitta et al., 2010).
3.3. Modification of Bacterial Cellulose
The process of modifying large quantities of natural fibers with BC was investigated, and the adhesion between the modified fibers and renewable polymers such as cellulose acetate butyrate and poly(L-lactic acid) was quantified by employing the single fiber pullout test (Bodin, 2010), providing new ideas for the modification of BC. Natural fibers have been modified for the reinforcement of polymers, for example by producing a diblock copolymer of BC and poly(methyl methacrylate) (BC-block-PMMA) through the mechanical fracture of BC with MMA (methyl methacrylate) in vacuum at 77 K. The radical polymerization of MMA was initiated by the mechanoradicals located on the BC surface, which was fully covered with the PMMA chains of the BC-block-PMMA (Sakaguchi et al., 2010).
A novel copolymer of polylactide and glycidyl methacrylate (PLA-co-PGMA) was prepared and used to modify the BC surface. PLA-co-PGMA was efficient at modifying the surface of BC nanofibrils and improving the compatibility of PLA/cellulose composites (Li et al., 2010). Moreover, polylactide-graft-methacryloxypropyltrimethoxysilane (PLA-g-MPS) was prepared by grafting MPS onto PLA, and then used to modify BC. The results revealed that the modified BC possessed a much more hydrophobic nature than virgin BC (Li et al., 2010).
3.4. Multiform Bacterial Cellulose
The field of application of BC synthesized by
Phase separation phenomena in aqueous suspensions of BC nanocrystals obtained by sulfuric acid hydrolysis have been studied. Suspensions at concentration above 0.42 wt % separated into isotropic and chiral nematic phases with a clear phase boundary. The size of the ordered domains in the anisotropic phase decreased with NaCl concentrations in the range from 0 to 2.75 mM. At 2.75 mM only tactoids were observed in the entire region, while at 5.0 mM, chiral nematic domains were no longer observed. The chiral nematic pitch decreased as the concentration of NaCl incvreased, reaching a minimum value at approximately 0.75 mM, and then increased sharply with the NaCl concentration up to 2.0 mM (Hirai et al., 2009). Obtaining a well-dispersed suspension is a prerequisite when preparing smooth model surfaces based on neutral bacterial cellulose nanocrystals (BCNs). However, neutral nanocrystal suspensions suffer from pronounced particle aggregation. Carboxymethyl cellulose (CMC) or xyloglucan (XG) were added to the aggregated BCN suspensions to minimize this problem. CMC enhanced the dispersion of BCN above a concentration ratio of 0.05. In the case of XG, enhanced colloidal stability was observed above a concentration ratio of 0.5. The results obtained demonstrated that cellulose-based model surfaces obtained by spin-coating from CMC/BCN or XG/BCN solutions exhibited a more uniform topography and less surface roughness than the reference unmodified BCN model surface (Winter et al., 2010).
4. Skin tissue repair materials from Bacterial Cellulose
Owing to its unique nano-scaled three-dimensional network structure, BC has a high water retention, high mechanical strength, and outstanding biocompatibility, which enable it to serve as a natural scaffold material for the regeneration of a wide variety of tissues (MacNeil, 2007; Siró, 2010; Klemm, 2006; Czaja, 2006). For most repair materials, important characteristic are their ability to lock exudate during the dressing process, as well as their removal from a wound surface after recovery. Traditionally, skin tissue repair materials have been absorbent, permeable materials. For example gauze, a traditional dressing material, can adhere to desiccated wound surfaces and induce trauma on removal of the dressing. Recently, interest in cellulose produced by bacteria from surface cultures has increased steadily because of its potential for application in medicine and cosmetics (Hornung et al., 2009). On one hand, its potential lies in the unique properties (such as the high mechanical strength) of the never-dried BC membrane; on the other hand, its high liquid absorbency, biocompatibility and hygienic nature perfectly cater to the specific demands for skin tissue repairing. Thus, considering the properties of BC as well as its clinical performance, the commercialization of BC for wound care is very promising (Czaja et al., 2006).
4.1. Basic properties of skin tissue repair materials
Compared to plant cellulose, BC has features such as a high crystallinity, tensile strength and water absorption capacity; good permeability; biocompatibility; resistance to degradation and a low solubility that may be advantageous features for skin tissue materials. The BC pellicle has an asymmetric structure composed of a fine network of nanofibrils similar to a collagen network. The shape of the stress-strain response curve of BC is reminiscent of the stress-strain response of the carotid artery, most probably due to the similar architecture of both types of nanofibrill networks (Backdahl et al., 2006). The freezable bound water behaves like water confined within pores rather than a typical polymer solvent, and it is possible to use the Gibbs-Thomson equation based on thermoporosimetry to obtain information on the pore structure of BC. In comparison with nitrogen adsorption, it was found that thermoporosimetry underestimated the porosity of BC, which may be due to a large non-freezable water fraction interacting with cellulose (Kaewnopparat et al., 2008).
The water vapor permeability of air-dried BC is quite excellent because of the presence of a large number of hydroxyl groups. BC membranes are highly selective to water; the highest selectivity observed [(p) = 186] was obtained for a mixture of trihydric alcohol viz. glycerol (Gly) with 40% (v/v) water. The binary system of monohydric alcohol viz. ethanol (EtOH) and water (40% (v/v)) showed the lowest selectivity [(p) = 12] but the highest pervaporative flux of 614 gm-2h at 35 oC, which further increased to 1429 gm-2h at 75 oC. However, the selectivity also decreased to 1.3 with the increase in temperature. The pervaporation behaviour was interpreted in terms of sorption and diffusivity of the organics, which in turn was influenced by the extent of their hydrogen bonding with the cellulose units in the membrane and the plasticization induced by the permeating water present in the binary mixture (Pandey et al., 2005).
4.2. Biocompatibility of skin tissue repair materials
BC is advantageous as engineered skin tissue material. However, little information is available concerning the potential toxicity of BC-based biomaterials. The toxicity of BC nanofibers was evaluated
After co-culture with fibroblasts (FB) and chondrocytes, respectively, BC compositions were implanted into nude mice. The BC co-culture composition was well integrated into the skin of nude mice. Thus, it is natural to conclude that BC was beneficial to cell attachment and proliferation under these conditions (Wang et al., 2009).
Helenius et al. implanted BC subcutaneously into rats and evaluated the implants with respect to chronic inflammation, foreign body responses, cell ingrowth, and angiogenesis through histology, immunohistochemistry, and electron microscopy. There were no macroscopic signs of inflammation around the implants: No fibrotic capsule or giant cells were present. Fibroblasts infiltrated BC, which was well integrated into the host tissue and did not elicit any chronic inflammatory reactions (Helenius et al., 2006). The
The attachment of cells to biomedical materials can be improved by utilizing adhesive amino acid sequences, such as Arg-Gly-Asp (RGD), found in several extracellular matrix proteins. To improve the cell biocompatibility of BC, Andrade et al. grafted RGD onto BC films that exhibited improved biocompatibility (Andrade et al., 2010). In order to enhance cell affinity, BC was also modified with nitrogen plasma. The treatment did not increase the wettability of the material, but increased its porosity and modified its surface chemistry, as demonstrated by the presence of nitrogen. The potential of plasma treatment for the surface modification of BC was demonstrated by Pertile et al. (Pertile et al., 2010). Specially, microporous BC scaffolds were seeded with urine-derived stem cells, which were induced to differentiate into urothelial and smooth muscle cells (Bodin, 2010).
4.3. Composites of Bacterial Cellulose
While BC can be used as skin tissue repair material, it has no significant influence on the biochemical state of chronic wounds. To improve the positive features of BC as wound dressing material, it was modified by the incorporation of collagen type I into a cellulose pellicle. The modified biomaterial was able to reduce the adsorbed amounts of certainproteases and interleukins significantly and possessed a distinct antioxidant capacity as well (Wiegand et al., 2006).
Double-network (DN) hydrogels with high mechanical strength were synthesized from BC and gelatin. The fracture strength and elastic modulus of a BC-gelatin DN gel under compressive stress were on the order of megapascals, which is several orders of magnitude higher than for a gelatin gel, and almost equivalent to articular cartilage. Similar enhancement in the mechanical strength was also observed for a combination of BC with polysaccharides such as sodium alginate, gellan gum, and i-carrageenan (Nakayama et al., 2004). For example, the membrane with 80 wt % BC/20 wt % alginate displayed a homogeneous structure and exhibited enhanced water adsorption capacity and water vapor transmission rate. Supercritical carbon dioxide drying was used for the formation of a nanoporous structure. However, the tensile strength and elongation at break of a film with a thickness of 0.09 mm decreased to 3.38 MPa and 31.60%, respectively. The average pore size of the blend membrane was 10.6 Å with a 19.5 m2/g specific surface area (Phisalaphong et al., 2008). Beside the composite with alginate, BC and gelatin were also selected to prepare membranes and the morphology of Swiss mouse embryo fibroblast NIH/3T3 cells grown on the surface of these membranes was examined to select the best material for the development of a biodegradable skin tissue regeneration template. Membranes derived cow bone gelatin and fish skin gelatin were stronger and more flexible than those prepared from pork skin gelatin in their wet forms (Nwe et al., 2010).
To develop functional property, a freeze-dried BC film was immersed in a benzalkonium chloride solution, a cationic surfactant and antimicrobial agent, followed by another freeze-drying step. It was showed that the drug-loading capacity of the BC dry film was about 0.116 mg/cm2 when soaked in 0.102% benzalkonium chloride solution (Fig. 2). As to the antimicrobial activity, a stable and prolonged activity was observed for at least 24 h, especially against
BC was formed and coated on cotton gauze samples during its biosynthesis. The composite obtained displayed more than 30% increase in water absorbency and wicking ability, and a 33% reduction in drying time as compared to untreated gauze (Meftahi et al., 2010).
The interactions between BC fibrils and aloe vera gel were investigated by Saibuatong et al. With a 30% v/v aloe gel supplement in the culture medium, the fibre-reinforced bio-polymer film obtained displayed significantly improved properties in terms of mechanical strength, crystallinity, water absorption capacity, and water vapor permeability in comparison to unmodified BC films. The average pore size of the modified films either in the dry or re-swollen form was decreased to approximately 1/5 of the unmodified BC films, while a narrow pore size distribution was maintained (Saibuatong et al., 2010).
BC/poly (ethylene glycol) (PEG) composites were prepared by immersing wet BC pellicle in PEG aqueous solutions followed by freeze-drying. Scanning electron microscope (SEM) images showed that the PEG molecules not only coated on the BC fibrils surface but also penetrated into the BC fiber network. It was found that PEG affected the preferential orientation of the plane during drying of the BC pellicle, which in turn decreased the crystallinity of the dried BC film. Thermogravimetric analysis (TGA) results showed that the thermal stability was improved from 263 to 293 degrees C, which may be associated with strong interactions between BC and PEG. Biocompatibility of the composite was preliminarily evaluated by cell adhesion studies using 3T3 fibroblast cells. Incubation of the cells with the BC/PEG scaffolds accelerated cell adhesion and proliferation (Cai et al., 2010). Various BC composites have displayed enhanced applicability as skin tissue repair materials (Table 1).
|Collagen||Reduced sorption of proteases and interleukins||Wiegand et al., 2006|
|Enhanced mechanical strength||Nakayama et al., 2004|
|Alginate||Changed tensile strength and elongation at break||Phisalaphong et al., 2008; New et al., 2010|
|Stable and prolonged antimicrobial activity|
Decreased crystallinity, improved thermal stability
|Wei et al., 2011|
Cai et al., 2010
|Cotton gauze||Increased water absorbency, wicking and water retention ability||Meftahi et al., 2010|
|Aloe vera gel||Improved mechanical strength, crystallinity, water sorption capacity, and water vapor permeability||Saibuatong et al., 2010|
4.4. Nano-composites of Bacterial Cellulose and Ag
BC is an optimal material for skin tissue repair since it provides a moist environment to a wound, which is beneficial to healing. Unfortunately, BC itself has no antimicrobial activity to prevent wound infection. To achieve antimicrobial activity, silver nanoparticles and chitosan were combined with BC. Due to the electron-rich oxygen atoms in the BC macromolecules and the large surface area of nanoporous BC effective as nanoreactor, the
The composite was obtained by immersing BC in a silver nitrate solution, and sodium borohydride was used to reduce the absorbed silver ions (Ag+) inside of BC to metallic silver nanoparticles (Fig.3). A red-shift and broadening of the optical absorption band was observed. The freeze-dried silver nanoparticle-impregnated BC exhibited strong antimicrobial activity against
With absorbed silver nanoparticles and stabilized by N-polyvinylpyrrolidone, inhomogeneous nanoparticle in the BC gel film were synthesized. The dried composite had large particles located on the layer surface of cellulose (Volkov et al., 2009). Colloidal submicron Ag particles were prepared on BC
To obtain the composite of BC and Ag, an ion exchange of the sodium to the silver salt was performed in an AgNO3 solution, followed by thermal reduction. By using oxidized BC nanofibers as a reaction template, stable silver nanoparticles were prepared with a narrow size distribution and a high density, through strong ion interactions between the host carboxylate groups from BC and guest silver cations (Ifuku et al., 2009). The
A facile method was developed to prepare a magnetic Ag nanocomposite. The 3D nanofibrous structure of BC was first homogenized with a ferric and ferrous salt mixture on a high speed blender. The magnetite nanoparticles were precipitated and incorporated into the BC nanostructures by adjusting the homogenate to alkaline pH. The magnetic BC nanofiber, when soaked in dopamine solution, can be coated with an adherent self-polymerized polydopamine layer. Since the polydopamine surface is very effective for reducing the silver ion, Ag nanoparticles were incorporated into the dopamine-treated magnetic BC by soaking in silver nitrate solution. The magnetization of the as-prepared Ag nanocomposite was maintained, and the magnetic Ag nanocomposite possessed a high antimicrobial activity against the model microbes
4.5. Nano-composite of Bacterial Cellulose and chitosan
Nanocomposite films based on different chitosan matrices (chitosans with two different degrees of polymerization and one water-soluble derivative) and BC were prepared by casting the water-based suspension of chitosan and BC nanofibrils, which is a fully “green” procedure. The films were highly transparent, flexible, and displayed better mechanical properties than the corresponding unfilled chitosan films (Fernandes et al., 2009). BC/chitosan composite materials showed a high sensitivity to enzymatic degradation and bioactivity. This innovatively modified BC nevertheless represents a good value for biomedical applications (Ciechanska, 2004). The potential of chitosan/BC was compared with that of the parent polymers and with chitosan/poly(vinyl alcohol) blends (Dubey et al., 2005).
By varying the chitosan concentration and immersion time, a foam-like structure was obtained. With increasing chitosan content, the crystalline structure remained unchanged, but the crystallinity index tended to decrease. The tensile strength and Young's modulus of the composites tended to decrease with increasing chitosan content but the values were much higher than for pure chitosan (Cai et al., 2009). A family of polysaccharide-based BC/chitosan porous scaffold materials with various weight ratios (from 20/80 to 60/40 w/w %) were prepared by freezing (-30 and -80 degrees C) and lyophilization of a mixture of microfibrillated BC suspension and chitosan solution. The microfibrillated BC (MFC) was subjected to 2,2,6,6-tetramethylpyperidine-1-oxyl radical (TEMPO)-mediated oxidation to introduce surface carboxyl groups before mixing. The composite scaffolds had a three-dimensional open pore microstructure with pore sizes ranging from 120 to 280 μm with enhanced compressive moduli and strength (Nge et al., 2010).
4.6. Clinical treatment
Following standard care, nonhealing lower extremity (LE) ulcers were treated with a BC wound dressing, Dermafill TM, (AMD/Ritmed, Tonawanda, NY). The time required for 75% reduction in wound size was compared for 11 chronic wounds without and with the application of BC. The mean period of observation without the application of BC was 315 days; (95% CI: 239-392 days). With the application of BC to these chronic wounds, the mean time for 75% epithelization was reduced to 81 days (95% CI 50-111 days) with a median value of 79 days. When applied to nonhealing LE ulcers, a BC wound dressing clearly shortens the time to wound closure over standard care (Portal et al., 2009).
Clinical trials were conducted on 34 patients suffered from severe thermal burns (second-degree A/B) covering 9–18% of the total body surface area (TBSA), 22 of the patients received the BC as testing group. The adherence of BC membrane to the wound surface was excellent to avoid any dead spaces because of its high conformability, and none of the patients using BC wound dressing during the trial developed any kind of hypersensitive reactions. By the tenth day of the treatment period, the process of reepithelialization had begun in 7 patients from the testing group (58.3%) in comparison with 4 patients (33.3%) from the control group. These results show that the application of BC dressing in the treatment of partial thickness burns promotes the creation of a favorable environment for fast wound cleansing, and consequently its rapid healing. It is worth mentioning that the release of the dressing from the wound was an entirely painless operation, due to the moisture still present in the never-dried cellulose structure ( Czaja et al., 2007).
The conformability and elastic properties of BC dressing allowed a high degree of adherence to the wound sites, even to the moving parts like hands (Fig. 4), torso, faces (Fig. 5) and so on. A complete closure of the wounded face with a single sheet of BC in which the holes for eyes, nose, and mouth were made after placement has been applied to a patient with the severe deep second-degree burns of the facial surface. After 44 days, the wounded face was entirely healed with no need for skin grafting and no significant signs of extensive scarring (Czaja et al., 2007).
In a randomized trial on predominantly category II and III skin tears in a population of frail elderly nursing home residents, standard wound care (24 residents) with XeroformTM and a secondary dressing (TegadermTM) was compared with a single application of BC Dermafill (27 residents). Outcomes included a decrease in the time to wound closure, pain reduction, and ease of use. Even though the wound area was slightly larger in the BC-treated group, the healing time was equivalent to the controls. However pain control, ease of use, and patient and nursing staff satisfaction were superior to the control experiments with the use of the BC skin tissue repair materials (Solway et al., 2010). Another test compared the rate of wound healing in diabetic foot ulcers (DFU) using either BC wound dressing or XeroformTM Petrolatum gauze. In a parallel, open-label trial in which the primary outcome was the rate of wound healing and the time to wound closure, 15 ulcers in type II diabetic patients received a BC dressing. Wounds in 19 control patients with type II diabetes were treated with a XeroformTM gauze dressing. All wounds were non infected Wagner stage II or III and received standard care including debridement, non-weight bearing limb support and weekly wound evaluation. With the provision of current care standards, the application of a BC dressing to a diabetic ulcer enhanced the rate of wound healing and shortened the epithelisation time (Solway et al., 2011). All treatments showed that using BC dressings or films was easy to manage because the patients exhibited a rapid rate of closure with the treatment. Therefore, clinical treatment with BC skin tissue repair materials can be considered an efficient method to treat acute and chronic wounds.
|Bacterial cellulose hydrogel|
Bacterial cellulose-nano silver
bacterial cellulose membrane
Metalized bacterial cellulose
Bacterial cellulose network, cationic polymer
Construction of fuel cells, electronic devices
Personal cleansing compositions
Cultural relics conservation
Skin tissue repair materials
|[ZL 201020239963.4] (Li et al, 2011)|
[ZL 200910149665.8] (Zhong, 2011)
[ZL 200810022130.X] (Xu et al, 2011)
[US 7,803,477 B2] (Evans et al., 2010), [US 2011 / 0014525 A1]  (Evans et al., 2011)
[US 2011 / 0039744 A1] (Heath et al., 2011)
[ZL 200810246345.X] (Wu et al, 2011)
[ZL 200810047793.7] (Yang et al., 2010)
|Patterned bacterial cellulose|
Novel bacterial cellulose
Poly(vinyl alcohol)- bacterial cellulose
Palladized bacterial cellulose
Bacterial cellulose network
modified bacterium cellulose
Artificial dura mater
Reductive conversion reactions
Liquid detergent composition
Carbon nanotube-like thin films, cathode material, batteries
|[ZL 200810047875.1] (Yang et al., 2010)|
[US 2010 / 0016575 A1] (Yang et al., 2010)
[ZL 200710015537.5] (Ma et al, 2010)
[US 2010 / 0126945 A1] (Patel & Suresh, 2010)
[US 2010 / 0210501 A1] (Caggioni et al., 2010)
[ZL 200810051298.3] (Yu et al, 2010)
[US 2009 / 0309072 A1] (Hwang et al., 2009)
|bacterial cellulose membrane||face mask||[ZL 200610075040.8] (Zhong, 2008)|
Novel bacterial cellulose
Poly(vinyl alcohol)- bacterial cellulose nanocomposite
Soft tissue replacement, medical devices
Industry, clothes, medical supplies, food, functional materials
|[US 2007 / 0197779 A1] (Yang et al., 2007)|
[US 2007 / 0027108 A1] (Yang et al., 2007)
[US 2005 / 0037082 A1] (Wan. & Millon, 2005)
[US RE38,792 E] (Iguchi et al., 1988), [US 2004/ 0091978 A1] (Ishihara & Yamanaka, 2004), [US 2002/ 0065409 A1] (Ishihara & Yamanaka, 2002)
|Bacterial cellulose||Yield improvement in BC production||[6,132,998] (Naritomi et al., 2000)|
|Bacterial cellulose||Improvement of the properties of paper||[6,069,136] (Tahara et al., 2000)|
|Bacterial cellulose||In creased BC production rate and yield||[6,017,740] (Kouda et al., 2000)|
|Bacterial cellulose||Increased BC production rate||[6,013,490] (Kouda et al., 2000)|
|Enzymatic detergent drain cleaners||Removal or prevention of BC growth||[5,975,095] (Ahmed et al., 1999)|
|Gelationous bacterial cellulose||Production of soft and light fibers||[5,962,676] (Tammarate, 1999)|
|Reticulated bacterial cellulose||Coating on a substantially continuous basis, coated products||[5,637,197] (Watt et al., 1997)|
|Reticulated bacterial cellulose||Reinforced elastomeric articles, pneumatic tires||[5,290,830] (Tung et al., 1994)|
|Bacterial cellulose||Banding agent||[5,207,826] (Westland et al., 1993)|
|Purified bacterial cellulose||Binding- suspended cholesterol or cholesterol esters||[4,960,763] (Stephen et al., 1990)|
|Bacterial cellulose||Replacement for latex binders||[4,919,753] (Johnson & Neon, 1990)|
|Bacterial cellulose||Printing materials||[4,861,427] (Johnson et al., 1989)|
|Bacterial cellulose||Molding material||[4,742,164](Iguchi et al., 1988)|
Bacterial cellulose (BC) is a promising natural polymer with many applications, especially for skin tissue repairing. Many advantages of BC give it great potential in wound healing system, such as biocompatible, conformability, elasticity, transparency, ability to maintain a moist environment in the wound and absorb exudates during inflammatory phase, and so on. This chapter discussed the most recent developments in BC-based skin tissue repair materials, including their biosynthesis, methods of treatment, properties, and frontier research on BC skin tissue repair materials. The structure of native and modified BC having been studied intensively and biocompatibility having been evaluated, suggested that BC could function as a skin tissue repair material well. Different BC products having been successfully applied as skin tissue repair and wound dressing materials, confirmed this. In addition, BC could have other applications in wound healing and regenerative medicine, such as guided tissue regeneration, periodontal treatments, or as a replacement for dura mater (the membrane surrounding brain tissue). Last but not least, BC is valuable in tissue engineering applications including bone, cartilage, blood vessel engineering, and so on. In a conclusion, if BC can be successfully mass-produced, it will eventually become a vital biomaterial used in the creation of a wide variety of medical devices and consumer products.
It was supported by National Natural Science Foundation of China (20774033, 21074041), the Fundamental Research Funds for the Central Universities, Huazhong University of Science and Technology (2010JC016), and the Natural Science of Hubei Province for Distinguished Young Scholars (2008CDB279). The authors are also grateful Professor Mario Gauthier (University of Waterloo, Canada) and Mr. Bo Wang (University of Tennessee, USA) for their valuable suggestions during the preparation of this manuscript.
Ahmed F. U. Goldschmidt J. E. La Cosse G. E. 1999Enzymatic detergent composition and method degrading and removing bacterial cellulose and glycerides,
Bohn A. Fink H. P. Ganster J. Pinnow M. 2005Measurement of the elastic modulus of single bacterial cellulose fibers using atomic force microscopy,
Caggioni, M.; Ortiz, R.; Barnabas, F. A.; Nunes, R. V.; Flood, J. A.& Corominas, F. ( 2010) Liquid detergent composition comprising an external structuring system comprising a bacterial cellulose network,
Cai Z. Kim J. 2010Bacterial cellulose/poly (ethylene glycol) composite: characterization and first evaluation of biocompatibility,
Ciechanska D. 2004Multifunctional bacterial cellulose/chitosan composite materials for medical applications,
Biomedical Applications of Microbial Cellulose in Burn Wound Recovery. Brown, R. M.; Jr. and I.M. Saxena ( Czaja W. Krystynowicz A. Kawecki M. Wysota K. Sakiel S. Wróblewski P. Glik J. Nowak M. Bielecki S. 2007
Dubey V. Pandey L. K. Saxena C. 2005Pervaporative separation of ethanol/water azeotrope using a novel chitosan-impregnated bacterial cellulose membrane and chitosan-poly (vinyl alcohol) blends,
Evans B. R. O’Neill H. M. Jansen V. M. Woodward J. 2010Metalization of bacterial cellulose for electrical and electronic device manufacture,
Evans, B. R.; O’Neill, H. M.; Jansen, V. M.; Woodward, J. ( 2011). Metalization of bacterial cellulose for electrical and electronic device manufacture, US Patent 2011 / 0014525 A1
Heath, B. P.; Coffindaffer, T. W.; Kyte, K. E.; Smith, E. D. & McConaughy, S. D. ( 2011). Personal cleansing compositions comprising a bacterial cellulose network and cationic polymer, US Patent 2011 / 0039744 A1
Hwang, S.; Chen, H. & Hwang, B. ( 2009). Bacterial cellulose film and Carbon nanotubes-like thin film structures developed from bacterial cellulose, US Patent 2009 / 0309072 A1
Iguchi M. Mitsuhashi S. Ichimura K. Nishi Y. Uryu M. Yamanaka S. Watanabe K. 1988Bacterial cellulose-containing molding material having high dynamic strength,
Iguchi M. Mitsuhashi S. Ichimura K. Nishi Y. Uryu M. Yamanaka S. Watanabe K. 1988Bacterial cellulose-containing molding material,
Iguchi M. Yamanaka S. Budhiono A. 2000Bacterial cellulose- a masterpiece of nature’s arts,
Ishihara, M. & Yamanaka, S. ( 2002). Modified bacterial cellulose, US Patent 2002/ 0065409 A1
Ishihara, M. & Yamanaka, S. ( 2004). Modified bacterial cellulose, US Patent 2004 / 0091978 A1
Johnson D. C. Neon A. N. Le Blanc H. A. 1989Bacterial cellulose as surface treatment foe fibrous web,
Johnson D. C. Neon A. N. 1990Nonwoven fabric-like product using a bacterial cellulose binder and method for its preparation,
Kouda T. Naritomi T. Yano H. Yoshinaga F. 2000Method for cultivation apparatus for the production of bacterial cellulose in an aerated and agitated culture,
Kouda T. Naritomi T. Yano H. Yoshinaga F. 2000Process for the production of Bacterial cellulose-containing molding material,
Li Z. Zhu B. J. Yang J. X. Peng K. Zhou B. H. Xu R. Q. Hu W. L. Chen S. Y. Wang H. P. 2011Method for manufacture of bacterial cellulose hydrogel cold pack,
Maria L. C. S. Santos A. L. C. Oliveira P. C. Valle A. S. S. Barud H. S. Messaddeq Y. Ribeiro S. J. L. 2010Preparation and Antibacterial Activity of Silver Nanoparticles Impregnated in Bacterial Cellulose.
Naritomi T. Kouda T. Naritomi M. Yano H. Yoshinaga F. 2000Process for continuously preparing bacterial cellulose,
Patel, U. & Suresh, S. ( 2010). Reactor for reductive conversion reactions using palladized bacterial cellulose, US Patent 2010 / 0126945 A1
Sakaguchi M. Ohura T. Iwata T. Takahashi S. Akai S. Kan T. Murai H. Fujiwara M. Watanabe O. Narita M. 2010Diblock Copolymer of Bacterial Cellulose and Poly(methyl methacrylate) Initiated by Chain-End-Type Radicals Produced by Mechanical Scission of Glycosidic Linkages of Bacterial Cellulose,
Stephen R. S. Westland J. A. Neogi A. N. 1990Method of using bacterial cellulose as a dietary fiber component,
Tahara N. Watanabe K. Hioki N. Morinaga Y. Hajouda T. Miyashita H. Shibata A. Ougiya H. 2000Bacterial cellulose concentrate and method for the treatment of the concentrate,
Tammarate P. 1999Method for the modification and utilization of bacterial cellulose,
Tung W. C. Tung D. A. Callandei D. D. Bauer R. G. 1994Reticulated bacterial cellulose reinforcement for elastomers,
Vander Hart. D. L. Atalla R. H. 1984Studies of Microstructure in Native Celluloses Using Solid-state13C NMR,
Wan, W. & Millon, L. ( 2005). Poly (vinyl alcohol)- bacterial cellulose nanocomposite,
Watt W. D. Adams T. N. Peterson G. D. Stephens R. S. Askew J. M. 1997Process of coating a substrate with reticulated bacterial cellulose,
Westland J. A. Stephens R. S. Johaston W. C. Rosenkrans H. J. 1993Bacterial cellulose binding agent,
Wu S. Q. Yang Z. W. Chen G. L. Fang B. S. Wang K. M. Chen H. Zhou R. H. Wan Z. Y. Wu H. Wei Y. F. Min Y. Jiang A. B. Liu C. J. Liang Y. Zhang Z. G. Liu F. Qiu Z. M. 2011Method for utilizing bacterial cellulose in protecting silk cultural relic,
Xu C. Y. Sun D. P. 2011Manufacture of membrane electrode of proton exchange fuel cell using bacterial fibers,
Yang G. Fu L. N. He F. Zhou P. Yu L. J. 2010
Yang G. Wang G. Liu B. F. Shi X. D. Chen X. F. (2010)． 2010A new approach for controllable bio-fabrication of patterned cellulose nano-fibers via micro-fluidic techniques,
Yang, Z. F.; Raczkjowski, R.; Rubic, L. B; Mazyck, M. J. & Deely, K.M. ( 2007). Bacterial cellulose-containing formulations, US
Yang, Z. F.; Raczkjowski, R.; Rubic, L. B; Mazyck, M. J. & Deely, K.M. ( 2007). Method for producing effective bacterial cellulose-containing formulations, US Patent 2007 / 0027108 A1
Yang, Z. F.; Raczkjowski, R.; Rubic, L. B; Mazyck, M. J. & Deely, K.M. ( 2010). Bacterial cellulose-containing formulations lacking a carboxymethyl cellulose component, US Patent 2010 / 0016575 A1
Yu D. Y. Qiao N. Zhang J. B. Guan X. H. Zhang J. Liu W. C. Yu J. 2010Method of preparing bacterium cellulose food-preserving film,
Zhong C. Y. 2008Bacterial cellulose gel face mask,
Zhong C. Y. 2011Method for manufacturing air-filtering bacterial cellulose face mask,
Andrade F. K. Moreira S. M. G. Domingues L. Gama F. M. P. 2010Improving the affinity of fibroblasts for bacterial cellulose using carbohydrate-binding modules fused to RGD,
Backdahl, H.; Helenius, G.; Bodin, A.; Nannmark, U.; Johansson, B. R.; Risberg, B. & Gatenholm, P. ( 2006). Mechanical properties of bacterial cellulose and interactions with smooth muscle cells, Biomaterials, 9 27 2141 2149
Baklagina Y. G. Khripunov A. K. Tkachenko A. A. Kopeikin V. V. Matveeva N. A. Lavrent’ev V. K. Nilova V. K. Sukhanova T. E. Smyslov R. Y. Zanaveskina I. S. Klechkovskaya V. V. Feigin L. A. 2005Sorption properties of gel films of bacterial cellulose,
Bielecki S. Krystynowicz A. Turkiewicz M. Kalinowska H. 2005Bacterial Cellulose,
Bodin A. Bharadwaj S. Wu S. Gatenholm P. Atala A. Zhang Y. 2010Tissue-engineered conduit using urine-derived stem cells seeded bacterial cellulose polymer in urinary reconstruction and diversion,
Bohn, A.; Fink, H. P.; Ganster, J. & Pinnow, M. ( 2000). X-ray texture investigations of bacterial cellulose, Macromolecular Chemistry and Physics, 15 201 1913 1921
Cai, Z.; Chen, P.; Jin, H. J. & Kim, J. ( 2009). The effect of chitosan content on the crystallinity, thermal stability, and mechanical properties of bacterial cellulose-chitosan composites, Proceedings of the Institution of Mechanical Engineers Part C-Journal of Mechanical Engineering Science, 10 223 2225 2230
Chawla P. R. Bajaj I. B. Survase S. A. Singhal R. S. (2009 2009Microbial Cellulose: Fermentative Production and Applications,
Czaja W. K. Young D. J. Kawecki M. Brown R. M. 2007The future prospects of microbial cellulose in biomedical applications,
Czaja W. Krystynowicz A. Bielecki S. Brown R. J. 2006Microbial cellulose- the natural power to heal wounds,
Czaja W. Romanovicz D. Brown R. M. 2004Structural investigations of microbial cellulose produced in stationary and agitated culture,
Dahman Y. 2009Nanostructured Biomaterials and Biocomposites from Bacterial Cellulose Nanofibers,
El -Saied H. Basta A. H. Gobran R. H. 2004Research progress in friendly environmental technology for the production of cellulose products (bacterial cellulose and its application),
Fernandes, S. C. M.; Oliveira, L.; Freire, C. S. R.; Silvestre, A. J. D.; Neto, C. P.; Gandini, A.; Desbrieres, J. ( 2009). Novel transparent nanocomposite films based on chitosan and bacterial cellulose, Green Chemistry, 12 11 2023 2029
Gelin K. Bodin A. Gatenholm P. Mihranyan A. Edwards K. Stromme M. 2007Characterization of water in bacterial cellulose,
Grande C. J. Torres F. G. Gomez C. M. Troncoso O. P. Canet-Ferrer J. Martinez-Pastor J. 2009Development of self-assembled bacterial cellulose-starch nanocomposites,
Helenius G. Backdahl H. Bodin A. Nannmark U. Gatenholm P. Risberg B. 2006In vivo biocompatibility of bacterial cellulose,
Hirai A. Inui O. Horii F. Tsuji M. 2009Phase Separation Behavior in Aqueous Suspensions of Bacterial Cellulose Nanocrystals Prepared by Sulfuric Acid Treatment,
Hornung M. Biener R. Schmauder H. P. 2009Dynamic modelling of bacterial cellulose formation,
Hsieh Y. C. Yano H. Nogi M. Eichhorn S. J. 2008An estimation of the Young’s modulus of bacterial cellulose filaments,
Hu W. L. Chen S. Y. Li X. Shi S. A. K. Shen W. Zhang X. Wang H. P. 2009In situ synthesis of silver chloride nanoparticles into bacterial cellulose membranes,
Hu Y. Catchmark J. M. 2010Formation and Characterization of Spherelike Bacterial Cellulose Particles Produced by
Ifuku S. Tsuji M. Morimoto M. Saimoto H. Yano H. 2009Synthesis of Silver Nanoparticles Templated by TEMPO-Mediated Oxidized Bacterial Cellulose Nanofibers,
Jeong S. I. Lee S. E. Yang H. Jin Y. H. Park C. S. . Park Y. S. 2010Toxicologic evaluation of bacterial synthesized cellulose in endothelial cells and animals,
Kaewnopparat S. Sansernluk K. Faroongsarng D. 2008Behavior of freezable bound water in the bacterial cellulose produced by Acetobacter xylinum: An approach using thermoporosimetry,
Klemm D. Heublein B. Fink H. P. Bohn A. 2005Cellulose: fascinating biopolymer and sustainable raw material,
Klemm D. Schumann D. Kramer F. Hessler N. Hornung M. Schmauder H. P. Marsch S. 2006Nanocelluloses as innovative polymers in research and application,
Kouda T. Yano H. Yoshinaga F. Kaminoyama M. Kamiwano M. 1996Characterization of non-Newtonian behavior during mixing of bacterial cellulose in a bioreactor,
Li Z. Q. Zhou X. D. Pei C. H. 2010Synthesis and Characterization of MPS-g-PLA Copolymer and its Application in Surface Modification of Bacterial Cellulose,
Li Z. Q. Zhou X. D. Pei C. H. 2010Synthesis of PLA-co-PGMA Copolymer and its Application in the Surface Modification of Bacterial Cellulose,
Lynd L. R. Weimer P. J. van Zyl W. H. Pretorius I. S. 2002Microbial cellulose utilization: Fundamentals and biotechnology,
Ma X. Wang R. M. Guan F. M. Wang T. F. 2010Artificial dura mater made from bacterial cellulose and polyvinyl alcohol,
Mac Neil. S. 2007Progress and opportunities for tissue-engineered skin.
Maneerung T. Tokura S. Rujiravanit R. 2008Impregnation of silver nanoparticles into bacterial cellulose for antimicrobial wound dressing,
Maria L. C. D. Santos A. L. C. Oliveira P. C. Barud H. S. Messaddeq Y. Ribeiro S. J. L. 2009Synthesis and characterization of silver nanoparticles impregnated into bacterial cellulose,
Masuda K. Adachi M. Hirai A. Yamamoto H. Kaji H. Horii F. 2003Solid-state 13C and 1H spin diffusion NMR analyses of the microfibril structure for bacterial cellulose,
Mc Kenna B. A. Mikkelsen D. Wehr J. B. Gidley M. J. Menzies N. W. 2009Mechanical and structural properties of native and alkali-treated bacterial cellulose produced by
Meftahi A. Khajavi R. Rashidi A. Sattari M. Yazdanshenas M. E. . Torabi M. 2010The effects of cotton gauze coating with microbial cellulose,
Mendes P. N. Rahal S. C. Pereira-Junior O. C. M. Fabris V. E. Lenharo S. L. R. de Lima-Neto J. F. Landim-Alvarenga F. D. 2009In vivo and in vitro evaluation of an
Nakayama A. Kakugo A. Gong J. P. Osada Y. Takai M. Erata T. . Kawano S. 2004High mechanical strength double-network hydrogel with bacterial cellulose,
Nge T. T. Nogi M. Yano H. Sugiyama J. 2010Microstructure and mechanical properties of bacterial cellulose/chitosan porous scaffold,
Nwe N. Furuike T. Tamura H. 2010Selection of a biopolymer based on attachment, morphology and proliferation of fibroblast NIH/3T3 cells for the development of a biodegradable tissue regeneration template: Alginate, bacterial cellulose and gelatin,
Olsson R. T. Kraemer R. Lopez-Rubio A. Torres-Giner S. Ocio M. J. Lagaron J. M. 2010Extraction of Microfibrils from Bacterial Cellulose Networks for Electrospinning of Anisotropic Biohybrid Fiber Yarns,
Olsson R. T. Azizi Samir. M. A. S. Salazar-Alvarez G. Belova L. Str Öm. V. Berglund L. A. Ikkala O. Nogués J. Gedde U. W. 2010Making flexible magnetic aerogels and stiff magnetic nanopaper using cellulose nanofibrils as templates,
Ougiya H. Watanabe K. Matsumura T. Yoshinaga F. 1998Relationship between suspension properties and fibril structure of disintegrated bacterial cellulose,
Pandey L. K. Saxena C. Dubey V. 2005Studies on pervaporative characteristics of bacterial cellulose membrane,
Pertile R. A. N. Andrade F. K. Alves C. Gama M. 2010Surface modification of bacterial cellulose by nitrogen-containing plasma for improved interaction with cells,
Phisalaphong M. Suwanmajo T. Tammarate P. 2008Synthesis and characterization of bacterial cellulose/alginate blend membranes,
Pommet M. Juntaro J. Heng J. Y. Y. Mantalaris A. Lee A. F. Wilson K. Kalinka G. Shaffer M. S. P. . Bismarck A. 2008Surface modification of natural fibers using bacteria: Depositing bacterial cellulose onto natural fibers to create hierarchical fiber reinforced nanocomposites,
Portal O. Clark W. A. Levinson D. J. 2009Microbial Cellulose Wound Dressing in the Treatment of Nonhealing Lower Extremity Ulcers,
Putra A. Kakugo A. Furukawa H. Gong J. P. Osada Y. Uemura T. Yamamoto M. 2008Production of bacterial cellulose with well oriented fibril on PDMS substrate,
Retegi A. Gabilondo N. Pena C. Zuluaga R. Castro C. Ganan P. de la Caba K. Mondragon I. 2010Bacterial cellulose films with controlled microstructure-mechanical property relationships,
Saibuatong O. A. Phisalaphong M. 2010Novo aloe vera-bacterial cellulose composite film from biosynthesis,
Sano, M. B.; Rojas, A.D.; Gatenholm, P. & Davalos, R. V. ( 2010). Electromagnetically Controlled Biological Assembly of Aligned Bacterial Cellulose Nanofibers, Annals of Biomedical Engineering, 8 38 2475 2484
Schrecker S. T. Gostomski P. A. 2005Determining the water holding capacity of microbial cellulose,
Shah J. Brown R. M. 2005Towards electronic paper displays made from microbial cellulose,
Shah N. Ha J. H. Park J. K. 2010Effect of Reactor Surface on Production of Bacterial Cellulose and Water Soluble Oligosaccharides by
Siró I. Plackett D. 2010Microfibrillated cellulose and new nanocomposite materials: a review,
Solway D. R. Clark W. A. Levinson D. J. 2011A parallel open-label trial to evaluate microbial cellulose wound dressing in the treatment of diabetic foot ulcers,
Solway D. R. Consalter M. Levinson D. J. 2010Microbial Cellulose Wound Dressing in the Treatment of Skin Tears in the Frail Elderly,
Sourty E. Ryan D. H. Marchessault R. H. 1998Ferrite-loaded membranes of microfibrillar bacterial cellulose prepared by in situ precipitation,
Sourty E. Ryan D. H. Marchessault R. H. 1998Characterization of magnetic membranes based on bacterial and man-made cellulose,
Sureshkumar M. Siswanto D. Y. Lee C. K. 2010Magnetic antimicrobial nanocomposite based on bacterial cellulose and silver nanoparticles,
Tamai N. Aono H. Tatsumi D. Matsumoto T. 2003Differences in rheological properties of solutions of plant and bacterial cellulose in LiCl/N,N-dimethylacetamide,
Tomita Y. Tsuji T. Kondo T. 2009Fabrication of Microbial Cellulose Nanofiber Network Sheets Hydrophobically Enhanced by Introduction of a Heat-printed Surface,
Vitta S. Drillon M. Derory A. 2010Magnetically responsive bacterial cellulose: Synthesis and magnetic studies,
Volkov V. V. Klechkovskaya V. V. Shtykova E. V. Dembo K. A. Arkharova N. A. . Ivakin G. I. Smyslov R. Y. 2009Determination of the size and phase composition of silver nanoparticles in a gel film of bacterial cellulose by small-angle X-ray scattering, electron diffraction, and electron microscopy,
Wang Z. L. Jia Y. Y. Shi Y. Cong D. L. Chen Y. Y. Jia S. R. Zhou Y. L. 2009Research on Characterization and Biocompatibility of Nano-bacterial Cellulose Membrane,
Wei B. Yang G. A. Hong F. 2011Preparation and evaluation of a kind of bacterial cellulose dry films with antibacterial properties,
Wiegand C. Elsner P. Hipler U. C. Klemm D. 2006Protease and ROS activities influenced by a composite of bacterial cellulose and collagen type I in vitro,
Winter H. T. Cerclier C. Delorme N. Bizot H. Quemener B. Cathala B. 2010Improved Colloidal Stability of Bacterial Cellulose Nanocrystal Suspensions for the Elaboration of Spin-Coated Cellulose-Based Model Surfaces,
Yamanaka S. Watanabe K. Iguchi M. . Nishi Y. (1998 1998Production, property, and application of bacterial cellulose,
Yoshinaga F. Tonouchi N. Watanabe K. 1997Research progress in production of bacterial cellulose by aeration and agitation culture and its application as a new industrial material,